- Nano Express
- Open Access
Energetic Al/Ni Superlattice as a Micro-Plasma Generator with Superb Performances
Nanoscale Research Letters volume 13, Article number: 374 (2018)
In this study, energetic Al/Ni superlattice was deposited by magnetron sputtering. A micro-plasma generator was fabricated using the energetic Al/Ni superlattice. The cross-sectional micro-structure of the energetic Al/Ni superlattice was scanned by transmission electron microscopy. Results show that the superlattice is composed of Al layer and Ni layers, and its periodic structure is clearly visible. Moreover, the bilayer thickness is about 25 nm, which consists of about 15 nm Al layer and 10 nm Ni layer. The micro initiator was stimulated using a 0.22 μF capacitor charged at 2900–4100 V. The electrical behaviors were investigated by testing the current-voltage waveform, and the plasma generation was explored by ultra-high-speed camera and photodiode. The integrated micro generator exhibited remarkable electrical exploding phenomenon, leading to plasma generations at a small timescale. The plasma outputs reflected by flyer velocities were superior to that with a much thicker bilayer of 500 nm Al/Ni multilayer. The higher flyer velocity combined with Gurney energy model confirmed the chemical reaction of the Al/Ni superlattice structure contributed to plasma production in comparison with the Al/Ni multilayers. Overall, the energetic Al/Ni superlattice was expected to pave a promising avenue to improve the initiator efficiency at a lower energy investment.
Reactive multilayer foils (RMFs) contain stored chemical energy in the form of layer structures that undergo rapid energy release when stimulated by an external energy source [1,2,3,4,5]. The reaction velocity and temperature of these foils are closely related to the composition and geometry [6,7,8,9]. They are potential for materials welding [10,11,12], explosive initiation [13,14,15], and biological neutralization .
Among the numerous existing RMFs, Al/CuO , Al/MoO3 , Al/PTFE , B/Ti , and Al/Ni [21, 22] are most extensively studied. Al/Ni RMFs exhibits superiority due to their high reaction heat (330 cal/g), outstanding fabrication quality, and cost efficiency. Many works have been conducted to reveal the thermodynamics properties and the exothermic self-sustained reaction performances of Al/Ni RMFs [23,24,25,26]. Results implicates that the reaction performances (e.g., maximum combustion temperature, combustion delay time) of Al/Ni RMFs depend strongly on their bilayer thickness . The RMFs with thinner bilayers have enhanced fuel/oxidizer interfacial contact areas and reduced average atomic diffusion distances so as to promote chemical reaction initiation . Meanwhile, the reaction velocity and temperature increases as the bilayer thickness decreases. However, when the bilayer thickness of RMFs is below 20 nm, a contrary trend is found due to a large degree of intermixed region .
When the bilayer thickness of the Al/Ni RMFs is decreased to molecular or sub-nanometer scale, an energetic Al/Ni superlattice is formed. Energetic Al/Ni superlattice presents unique chemical reaction properties due to extremely short distances among reactants, and relatively large intermixed region. The chemical reaction of energetic Al/Ni superlattice was characterized by various methods (differential scanning calorimetry , transmission electron microscopy , and time-resolved X-ray microdiffraction ) to better understand the chemical reaction mechanism. Results indicated that metastable phase was not formed for superlattice structure due to its extremely low diffusion distance .
Extensive works have been carried out referring to the combustion characteristics and chemical mechanism of energetic Al/Ni superlattice. However, there are lack of reports on the electrical behaviors and plasma performances based on the energetic Al/Ni superlattice under extra electrical stimulation. In the present study, energetic Al/Ni superlattice was deposited on Al2O3 substrates by magnetron sputtering and patterned by wet etching to form a plasma generator. The electrical behaviors and plasma performance of the generator under electrical stimulation were investigated in detail.
Energetic Al/Ni superlattice samples were fabricated by alternately depositing a layer composed of Al and Ni on Al2O3 substrates from Ni (99.99 wt%) and Al (99.99 wt%) targets. The base pressure of the deposition chamber was 5 × 10−5 Pa, and sputtering was performed with a process gas of Ar at pressures of 0.8 Pa. Both Al and Ni layer were deposited at 90 W. On above depositing conditions, the deposition rate for Al and Ni was about 15 nm/min and 10 nm/min, respectively. The bilayer thickness of as-deposited energetic Al/Ni superlattice was about 25 nm, and the overall thickness was about 4 μm. Each bilayer consisted of an Al layer and a Ni layer with a thickness ratio of 3:2 to maintain an overall 1:1 atomic ratio. As the comparison samples, Al/Ni RMFs with bilayer thickness of 500 nm were also deposited. The copper layer with thickness of 20 nm was deposited onto samples in order to keep good attachment to ceramic plug.
The fabrication process of the micro-plasma generator was based on the MEMS technique, as shown in Fig. 1. Firstly, 0.5-mm-thick 4-in. Al2O3 substrate was cleaned with acetone, alcohol, and deionized water in an ultrasonic bath for 5 min, respectively. Secondly, the substrates were dried in an oven for 30 min at 100 °C. Thirdly, the substrates were fixed on the specimen holder and their surface contaminants were removed by oxygen plasma. Then, energetic Al/Ni superlattice was deposited on the surface of Al2O3 substrate. Subsequently, a positive photoresist (AZ5214E) was spin-coated on the surface of as-deposited samples at 5000 rpm for 60 s and pre-baked in an oven for 90 s at 100 °C. Afterwards, the samples were patterned and exposed to an ultraviolet radiation with an intensity of 16 mJ/cm2. Later, the samples were developed in NaOH solution. The samples were again baked at 120 °C to stabilize the photoresist pattern. Finally, the samples were etched to form a bowtie bridge in Al etchant solution (Aluminum Etchant Type A, Transene Company, Danvers, Massachusetts) at 30 °C. The patterned samples were diced into multiple individual chips, and the remaining photoresist was removed in acetone. Lastly, the chip was assembled into a ceramic plug to form the plasma generator.
The cross-sectional structure of the plasma generator was characterized by the transmission electron microscopy (TEM). Subsequently, the micro-plasma generator was stimulated using a high-pulse current generator (0.22 μF, 2900–4100 V), and the current-voltage waveforms were measured using a Rogowski coil and a high-voltage probe, which recording by an oscilloscope. In the meantime, the plasma generation was recorded by a high-speed camera (SIM, SIL3001-00-H06). The exposure time of ultra-high-speed camera was 10 ns, and the interval time of each frame was about 20 –50 ns. In addition, the generating light intensity was measured by a photodiode. The testing baseline delay between the high-pulse current generator, ultra-high speed camera, and oscilloscope was controlled by a digital delay generator (DG535), which is shown in Fig. 2.
Furthermore, the performances of the micro-plasma generator were characterized by testing its ability to drive the Kapton flyer with the thickness of 30 μm. A short current pulse was applied on the plasma generator, causing a fast explosion of the bowtie bridge (0.4 × 0.4 mm), which in turn compelled the flyer to accelerate to a velocity up to several kilometer per second [33,34,35]. And the velocity of the flyer was recorded by a photonic Doppler velocimetry (PDV).
Results and Discussion
Figure 3a shows the cross-sectional bright-field TEM image of the energetic Al/Ni superlattice, which indicates a periodic structure consisting of Al and Ni bilayers with a controlled thickness, and different layers can be easily distinguished. The selected area electron diffraction (SAED) is further performed, as shown in Fig. 3b, c. The bright image corresponds to the Al layer, whereas the dark image denotes the Ni layer. The bilayer thickness is about 25 nm, which consist of about 15 nm Al layer and 10 nm Ni layer. The rings of diffraction indicate a well-defined polycrystalline structure of the Ni and Al layer. Figure 3d shows the cross-sectional bright-field TEM image of Al/Ni multilayers with a 500 nm bilayer thickness.
Figure 4a illustrates the voltage, current, light intensity, and energy histories of energetic Al/Ni superlattice charged at 3.5 kV. The evolution of voltage-current exhibits peaks of current and voltage. When a current pulse is supplied to the superlattice Al/Ni materials, the film is locally heated up due to the Joule effect, resulting in a rapid rise in the temperature corresponding to a rise in voltage across the bridge [36, 37]. Eventually, the voltage is enhanced highly enough to induce a drop in current, where the resistance reaches a maximum. The vaporized and ionized material constructs a new path of low resistance to make the voltage to drop towards zero accompanying with the discharging current to a maximum value.
Figure 4b shows the plasma evolution of energetic Al/Ni superlattice captured by ultra-high-speed camera. The process of Joule heating, evaporation, and plasma generating and expanding is evident. According to Fig. 4, a blurring light is observed, and the voltage and current rises slowly, indicating a Joule heating process (≤ 168 ns). At 218 ns, the voltage is suddenly increased while the emitting light is distinct, and the area of the light is nearly the area of the bowtie bridge. This corresponds to the evaporation process of the energetic Al/Ni superlattice. When the voltage reaches its maximum at 258 ns, the explosion associated with plasma generation takes place following with intense light. After exploding, the plasma expansion towards ambient is apt to cause shock wave. Product particles which existed in the combustion of Al/Ni RMFs are not observed in this study, implicating that the explosion of energetic Al/Ni superlattice is uniform under high-pulse current . Therefore, the time of the voltage peak can be regarded as the delay time (Tb) (between the onset of the current pulse and the voltage peak signal). The energy absorbed of the sample during this delay time is deemed as the critical explosion energy (Ec). We should note that the point of onset light emission intensity corresponds to the voltage peak (258 ns). The signal of light emission intensity is hardly to be detected because of the weak light prior to explosion.
The results of Tb and Ec are obtained from integrating electrical voltage-current curves under different charging voltage ranging from 2900 to 4100 V as presented in Fig. 5a. As shown in Fig. 5a, Tb decreases with the increase of charging voltage. According to the inset image in Fig. 5a, the maximum current reaches about 2572 A at 4100 V, whereas the current peak achieves 1870 A at 2900 V. It is indicated that the electrical energy input per unit time of energetic Al/Ni superlattice is increased with the increase of charging voltage. So, the delay time at lower charging voltage is much longer in comparison with high charging voltages. However, for Ec values, it exhibits an enhanced trend with the increase of charge voltage, implying that more electrical energy is absorbed to the point of exploding at 4100 V for energetic Al/Ni superlattice in comparison to that at 3500 and 2900 V, which can be ascribed to the exploding heterogeneity under an electrical pulse. When a high-current pulse is applied to energetic Al/Ni superlattice, the temperature of the four corners is much higher than that of other sections resulting in an explosion at a shorter time as shown on Fig. 5b. The difference between the exploding sections is diminished with increasing the charging voltage. Thus, the electrical exploding of energetic Al/Ni superlattice seems more homogeneous at 4100 V than those at lower charge voltages, accounting for the high exploding voltage and electrical energy.
Figure 6a shows the flyer velocities by plasma expansion at charging voltages ranging from 2900 to 4100 V for energetic Al/Ni superlattice. After the electrical pulse is loaded on the superlattice, the expanding plasma pressure accelerates the flyer away from the sample surface, causing a portion of the flyer to tear away and continue acceleration. As expected, the flyer velocity increases as the charging voltage is increased. For the charging voltage of 4100 V, the maximum flyer velocity achieves over 3 km/s, which is significantly higher than the peak value obtained at 3500 V charging voltage. When the charging voltage decreases to 2900 V, the flyer velocity is about 2.3 km/s.
The flyer velocity was measured three times at each charging voltage, and the maximum flyer velocity is averaged, as shown in Fig. 6b. Results show that the maximum flyer velocity of RMFs sample is much lower than that of energetic superlattice structures. Gurney energy model is introduced to reconcile different electrical energy and flyer-to-layers mass ratios between samples [39, 40]. The final flyer velocity is predicted according to:
where M is the flyer mass, B is the mass from which the plasma energy for acceleration comes, and Eg is the energy per unit mass provided to the system. K, n is the Gurney factor which is decided by composition and geometry of foil. Jb is the electrical exploding current density. In the current case, the samples have the same flyer-to-layer mass ratios and Gurney factor due to the identical bilayer thickness, total thickness, and geometry. The flyer velocity is related to electrical energy provided to the system (Eg), which is calculated by the exploding current density.
In our experiments results, the exploding current density of Al/Ni RMFs is higher than the superlattice. According to the Gurney energy model, the final flyer velocity of Al/Ni RMFs should exhibit a higher value in comparison to those samples integrated with energetic Al/Ni superlattice. But the predicted results are not consistent with experimental output (Fig. 6b). On the contrary, the experimental results with superlattice exhibit higher flyer velocity by contrasting RMFs. The increments of flyer kinetic energy confirm that the chemical energy generated from the reaction between Al and Ni is affected by the process of plasma for energetic Al/Ni superlattice. The heat release is attributed to high ionization of the superlattice during plasma formation process, resulting in a rapid plasma expansion velocity.
In this work, energetic Al/Ni superlattice was fabricated by alternatively deposited Al and Ni layer on the surface of Al2O3 ceramic substrates by magnetron sputtering, characterized by TEM. The electrical behaviors and plasma performances based on the energetic Al/Ni superlattice under extra electrical stimulation were investigated, which was integrated as a micro-plasma generator. The integrated micro generator exhibited remarkable electrical exploding phenomenon, leading to plasma generations at a small timescale. The plasma outputs reflected by flyer velocities were superior to that with a much thicker bilayer of 500 nm Al/Ni multilayer. The Gurney energy model confirmed that the chemical reaction of the Al/Ni superlattice structure was involved in the plasma generation in comparison with Al/Ni RMFs. Overall, the micro plasma generator based on energetic Al/Ni superlattice exhibits superior performance with high-plasma outputs, thus improving electrical energy transduction and system reliability. Hence, there is much prospect of the application of energetic Al/Ni superlattice on micro- or nano-plasma initiators to implement special function.
Reactive multilayer foils
Transmission electron microscopy
Kim JS, Lagrange T, Reed BW, Taheri ML, Armstrong MR, King WE, Campbell GH (2008) Imaging of transient structures using nanosecond in situ TEM. Science 321:1472–1475
Zhou X, Torabi M, Lu J, Shen R, Zhang K (2014) Nanostructured energetic composites: synthesis, ignition/combustion modeling, and applications. ACS Appl Mater Interfaces 6:3058–3074
Rossi C, Zhang K, Esteve D, Alphonse P, Tailhades P, Vahlas C (2007) Nanoenergetic materials for MEMS: a review. J Microelectromech Syst 16:919–931
Marin L, Nanayakkara CE, Veyan JF, Warot-Fonrose B, Joulie S, Esteive A, Tenailleau C, Chabal YJ, Rossi C (2015) Enhancing the reactivity of Al/CuO nanolaminates by Cu incorporation at the interfaces. ACS Appl Mater Interfaces 7:11713–11718
Adams DP (2015) Reactive multilayers fabricated by vapor deposition: a critical review. Thin Solid Films 576:98–128
Kuk SW, Ryu HJ, Yu J (2014) Effects of the Al/Ni ratio on the reactions in the compression-bonded Ni-sputtered Al foil multilayer. J Alloy Compd 589:455–461
Woll K, Gunduz IE, Pauly C, Doumanidis CC, Son SF, Rebholz C, Mucklich F (2015) Numerical modeling of self-propagating reactions in Ru/Al nanoscale multilayer foils. Appl Phys Lett 107:073103
Trenkle JC, Wang J, Weihs TP, Hufnagel TC (2005) Microstructural study of an oscillatory formation reaction in nanostructured reactive multilayer foils. Appl Phys Lett 87:153108
Rogachev AS (2008) Exothermic reaction waves in multilayer nanofilms. RussChem Rev 77:21–37
Wang J, Besnoin E, Duckham A, Spey SJ, Reiss ME, Knio OM, Powers M, Whitener M, Weihs TP (2003) Room-temperature doldering with nanostructured foils. Appl Phys Lett 83:3987–3989
Duckham A, Spey SJ, Wang J, Reiss ME, Weihs TP, Besnoin E, Knio OM (2004) Reactive nanostructured foil used as a heat source for joining titanium. J Appl Phys 96:2336–2342
Wang J, Besnoin E, Duckham A, Spey SJ, Reiss ME, Knio OM, Weihs TP (2004) Joining of stainless-steel specimens with nanostructured Al/Ni foils. J Appl Phys 95:248–256
Morris CJ, Wilkins P, May C, Zakar E, Weihs TP (2011) Streak spectrograph temperature analysis from electrically exploded Ni/Al nanolaminates. Thin Solid Films 520:1645–1650
Qiu X, Tang R, Liu R, Huang H, Guo S, Yu H (2012) A micro initiator realized by reactive Ni/Al nanolaminates. J Mater Sci Mater Electron 23:2140–2144
Morris CJ, Wilkins PR, May CM (2013) Streak spectroscopy and velocimetry of electrically exploded Ni/Al laminates. J Appl Phys 113:043304
Zhao S, Germann TC, Strachan A (2006) Atomistic simulations of shock-induced alloying reactions in Ni/Al nanolaminates. J Chem Phys 125:164707
Yang Y, Xu D, Zhang K (2012) Effect of nanostructures on the exothermic reaction and ignition of Al/CuOx based energetic materials. J Mater Sci 47:1296–1305
Xu J, Yu T, Ru C, Ji D, Ye Y, Shen R, Peng Z (2017) Tuning the ignition performance of a microchip initiator by integrating various Al/MoO3 reactive multilayer films on a semiconductor bridge. ACS Appl MaterInterfaces 9:5580–5589
Wang J, Jiang X, Zhang L, Qiao Z, Gao B, Yang G, Huang H (2015) Design and fabrication of energetic superlattice like-PTFE/Al with superior performance and application in functional micro-initiator. Nano Energy 12:597–605
Zhang YX, Wang Y, Ai MT, Jiang HC, Yan YC, Zhao XH, Wang L, Zhang WL, Li YR (2018) Reactive B/Ti nano-multilayers with superior performance in plasma generation. ACS Appl Mater Interfaces 10:21582–21589
Manukyan KV, Tan W, Deboer RJ, Stech E, Aprahamian A, Wiescher M, Weihs TP (2015) Irradiation-enhanced reactivity of multilayer Al/Ni nanomaterials. ACS Appl Mater Interfaces 7:11272–11279
Wang Y, Sun XJ, Jiang HC, Gao Y, Guo F, Wang L, Zhang YX, Fu QB (2018) Investigation of electrically heated exploding foils in reactive Al/Ni multilayer. Propellants Explos Pyrotech 43:1–7
Simoes S, Viana F, Ramos AS, Vieira MT (2010) TEM characterization of as-deposited and annealed Ni/Al multilayer thin film. Microsc Microanal 16:662–669
Grapes MD, Weihs TP (2016) Exploring the reaction mechanism in self-propagating Al/Ni multilayers by adding inert material. Combust Flame 172:105–115
Rogachev AS, Vadchenko SG, Mukasyan AS (2012) Self-sustained waves of exothermic dissolution in reactive multilayer nano-foils. Appl Phys Lett 101:063119
Blobaum KJ, Van Heerden D, Gavens AJ, Weihs TP (2003) Al/Ni formation reactions: characterization of the metastable Al9Ni2 phase and analysis of its formation. Acta Mater 51:3871–3884
Knepper R, Snyder MR, Fritz G, Fisher K, Knio OM, Weihs TP (2009) Effect of varying bilayer spacing distribution on reaction heat and velocity in reactive Al/Ni multilayers. J Appl Phys 105:083504
Gavens AJ, Van Heerden D, Mann AB, Reiss ME, Weihs TP (2000) Effect of intermixing on self-propagating rxothermic reactions in Al/Ni nanolaminate foils. J Appl Phys 87:1255–1263
Michaelsen C, Barmak K, Weihs TP (1997) Investigating the thermodynamics and kinetics of thin film reactions by differential scanning calorimetry. J Phys D Appl Phys 30:3167–3186
Maj L, Morgiel J (2017) In-situ transmission electron microscopy observations of nucleation and growth of intermetallic phases during reaction of Ni(V)/Al multilayers. Thin Solid Films 621:165–170
Trenkle JC, Koerner LJ, Tate MW, Walker N, Gruner SM, Weihs TP, Hufnagel TC (2010) Time-resolved x-ray microdiffraction studies of phase transformations during rapidly propagating reactions in Al/Ni and Zr/Ni multilayer foils. J Appl Phys 107:113511
Barmak K, Michaelsen C, Bormann R, Lucadamo G (1997) Reactive phase formation in sputter-deposited Ni/Al thin films. J Mater Res 12:133–146
Willey TM, Champley K, Hodgin R, Lauderbach L, Bagge-Hansen M, May C, Sanchez N, Jensen BJ, Lverson A, Van Buuren T (2016) X-ray imaging and 3D reconstruction of in-flight exploding foil initiator flyers. J Appl Phys 119:235901
Neal W, Bowden M (2017) High fidelity studies of exploding foil initiator bridges, part 2: experimental results. AIP Conference Proceedings 1793:030022
Zeng QX, Lv JJ, Li MY (2013) The influence of exploding foil shape on energy deposition. Rev Sci Instrum 84:066105
Morris CJ, Mary B, Zakar E, Barron S, Fritz G, Knio O, Weihs TP, Hodgin R, Wilkins P, May C (2010) Rapid initiation of reactions in Al/Ni multilayers with nanoscale layering. J Phys Chem Solids 71:84–89
Saxena AK, Kaushik TC, Gupta SC (2010) Shock experiments and numerical simulations on low energy portable electrically exploding foil accelerators. Rev Sci Instrum 81:033508
Taylor MJ (2002) Formation of plasma around wire fragments created by electrically exploded copper wire. J Phys D Appl Phys 35:700
Il'in AP, Nazarenko OB, Tikhonov DV, Ushakov VY (2002) Structural and energy processes in electrically exploded conductors. Russ Phys J 45:1176-1180
Kennedy JE (1998) The gurney model of explosive output for driving metal. In: Zukas JA, Walters W (eds) Explosive effects and applications. Springer, New York
We thank Dr. Binbin Liu at the University of Science and Technology Beijing for the support in providing materials characterization.
This work was supported by the basic research project fund of the central university (2672018ZYGX2018J023) and the china postdoctoral science fund (2018 M633344).
Availability of Data and Materials
Both authors declare that the materials, data, and associated protocols are available to the readers, and all the data used for the analysis are included in this article.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Wang, Y., Yan, Y., Jiang, H. et al. Energetic Al/Ni Superlattice as a Micro-Plasma Generator with Superb Performances. Nanoscale Res Lett 13, 374 (2018). https://doi.org/10.1186/s11671-018-2795-8
- Al/Ni Superlattice
- Micro-plasma generator
- Flyer velocity